Hot Electron Transistor with van der Waals Base-Collector Heterojunction and High-Performance GaN Emitter ... Publication Date (Web): April 17, 2017.
Apr 17, 2017 - ABSTRACT: Single layer graphene is an ideal material for the base layer of hot electron transistors (HETs) for potential terahertz (THz) ...
Apr 17, 2017 - School of Electrical and Computer Engineering, Cornell University, Ithaca, New York 14850, United States. â¥ Department of Physics, Massachusetts Institute of ... Citation data is made available by participants in Crossref's Cited-by
Mar 22, 2017 - Saudis advance chemicals from oil. In a move meant to diversify the Saudi economy beyond oil exports, SABIC and the Saudi national oil company... POLICY CONCENTRATES ...
16 mins ago - A; Accounts of Chemical Research · ACS Applied Bio Materials - New in 2018 · ACS Applied Energy Materials - New in 2018 · ACS Applied Materials & Interfaces · ACS Applied Nano Materials - New in 2018 · ACS Biomaterials Science & Enginee
28 Jun 2016 - Photovoltaic high-performance broadband photodetector based on MoS 2 /Si ... Fast, Self-Driven, Air-Stable, and Broadband Photodetector Based on ..... Oil and Gas Wastewater is a Cheap Fix for Road Dust but Comes at a Toxic Cost ... Aut
Van der Waals heterostructures built from two-dimensional materials on a conventional semiconductor offer novel electronic and optoelectronic properties for ...
Jun 28, 2016 - The WS2/Si heterojunction working in the Zener breakdown regime shows a stable and linear photoresponse, a broadband photoresponse ranging from 340 to 1100 nm with a maximum photoresponsivity of 5.7 A/W at 660 nm and a fast response sp
Materials Science & Technology Division, Naval Research Laboratory, Washington, DC 20375, USA a. Postdoctoral ... Engineering Education b. Postdoctoral .... In this image, there are two monolayer (ML) WSe2 triangles on top of hexagonal boron nitride
May 4, 2018 - In these structures, it is possible to create interlayer excitons (ILEs), spatially indirect, bound electronâhole pairs with the electron in one TMD ...
Subscriber access provided by Eastern Michigan University | Bruce T. Halle Library
Hot electron transistor with van der Waals base-collector heterojunction and high performance GaN emitter Ahmad Zubair, Amirhasan Nourbakhsh, Jing Yong Hong, Meng Qi, Yi Song, Debdeep Jena, Jing Kong, Mildred S. Dresselhaus, and Tomas Palacios Nano Lett., Just Accepted Manuscript • DOI: 10.1021/acs.nanolett.7b00451 • Publication Date (Web): 17 Apr 2017 Downloaded from http://pubs.acs.org on April 21, 2017
Just Accepted “Just Accepted” manuscripts have been peer-reviewed and accepted for publication. They are posted online prior to technical editing, formatting for publication and author proofing. The American Chemical Society provides “Just Accepted” as a free service to the research community to expedite the dissemination of scientific material as soon as possible after acceptance. “Just Accepted” manuscripts appear in full in PDF format accompanied by an HTML abstract. “Just Accepted” manuscripts have been fully peer reviewed, but should not be considered the official version of record. They are accessible to all readers and citable by the Digital Object Identifier (DOI®). “Just Accepted” is an optional service offered to authors. Therefore, the “Just Accepted” Web site may not include all articles that will be published in the journal. After a manuscript is technically edited and formatted, it will be removed from the “Just Accepted” Web site and published as an ASAP article. Note that technical editing may introduce minor changes to the manuscript text and/or graphics which could affect content, and all legal disclaimers and ethical guidelines that apply to the journal pertain. ACS cannot be held responsible for errors or consequences arising from the use of information contained in these “Just Accepted” manuscripts.
Hot electron transistor with van der Waals basecollector heterojunction and high performance GaN emitter Ahmad Zubair1*, Amirhasan Nourbakhsh1, Jin-Yong Hong1, Meng Qi2, Yi Song1, Debdeep Jena3, Jing Kong1, Mildred Dresselhaus1,4, Tomás Palacios1 1
Department of Electrical Engineering Computer Science, Massachusetts Institute of Technology, 77 Massachusetts Avenue, Cambridge, Massachusetts 02139, United States
Electrical Engineering Department, University of Notre Dame, Notre Dame, Indiana 46556, United States 3
School of Electrical and Computer Engineering, Cornell University, Ithaca, New York 14850, United States 4
Department of Physics, Massachusetts Institute of Technology, 77 Massachusetts Avenue, Cambridge, Massachusetts 02139, United States
KEYWORDS Hot Electron transistor, Graphene, GaN, WSe2, van der Waals heterostructure, Tunneling, Transition metal dichalcogenides ABSTRACT Single layer graphene is an ideal material for the base layer of hot electron transistors (HETs) for potential THz applications. The ultra-thin body and exceptionally long mean free path maximizes the probability for ballistic transport across the base of the HET. We demonstrate, for
the first time, the operation of a high performance HET using a graphene/WSe2 van der Waals (vdW) heterostructure as a base-collector barrier. The resulting device, with a GaN/AlN heterojunction as emitter, exhibits a current density of 50 A/cm2, DC current gain above 3 and 75% injection efficiency, which are record values among graphene-base HETs. These results not only provide a scheme to overcome the limitations of graphene-base HETs toward THz operation but are also the first demonstration of a GaN/vdW heterostructure in HETs, revealing the potential for novel electronic and optoelectronic applications.
The hot electron transistor1 is a promising device concept that could be used to overcome the limitations of heterojunction bipolar transistors (HBTs) and high electron mobility transistors (HEMTs) in ultra-high frequency applications. The HET is a unipolar and majority carrier device where the base-to-emitter voltage controls the transport of ballistic hot electrons through a transit layer smaller than the mean free path (λmfp) of the carriers. Hence, HETs have the potential to exhibit a superior high frequency performance relative to HBTs (limited by the diffusion of the minority carriers across the base) and HEMTs (limited by the saturation velocity of carriers and the lithography of the gate)1. As shown schematically in Figure 1a, a typical HET structure consists of a hot electron injector (emitter/emitter-barrier stack), a transport layer (base) and a hot electron analyzer or filter (collector-barrier/collector-stack). The HET can be considered as a combination of two back-to-back diodes connected in series, namely the E-B diode and the B-C diode. Under the operating conditions, the emitter-base (E-B) diode is forward biased (VBE > 0 V) and electrons are injected into the base with an excess energy above the Fermi energy of the
base (eVBE−Ef). If the base-collector (B-C) diode is then reverse biased (VCB > 0 V), it will allow the hot electrons reaching the base to travel to the collector with minimal scattering (quasiballistically) (Figure 1a). However, if VCB < 0 V, the energy barrier for the base electrons (shown by the dotted lines in Figure 1a) will increase and majority of the injected electrons will thermalize in the base by scattering and quantum mechanical reflection, and eventually contribute to the base leakage current. Several material systems have been used for HET development including metal thin films1, 2, non-polar III-V semiconductor heterostructures3-6, complex oxides7, and superconducting materials8. However, the successful demonstration of high performance HETs have been limited by the technological inability to scale the base thickness below the λmfp of the carriers and electrostatic decoupling of the collector from emitter. In the thick base regions used so far, the injected hot electrons are thermalized in the base as a result of inelastic (intra- and inter-valley6 electron–electron, electron–phonon) and elastic (impurities) scattering. To reduce inter-valley scattering, wide bandgap materials such as GaN have been recently used9,10, as they show large inter-valley separation. These GaN-based devices have demonstrated excellent current gain (>10)11 and current density (~kA/cm2)11,
temperature, however, similar to other bulk three-dimensional semiconductors, the growth of an ultra-scaled base layer still remains a challenge. Single atomic layer two-dimensional (2D) materials are naturally suitable for applications requiring ultra-thin, defect-free films. Several vertical tunneling devices13 for both logic (tunneling transistors14, barristors15) and high frequency applications (resonant tunneling device16) have been demonstrated using these materials. Monolayer graphene, with ultra-high mobility and a dangling-bond-free inert surface, is an ideal candidate as a low resistance, scattering-free base material in HETs that can overcome the growth-related limitations in bulk
semiconductors. Theoretical studies have predicted that with an optimized structure, a maximum unity gain operating frequency (fT) up to several THz17-21, Ion/Ioff over 105 and high current gain19, 22, 23 can be achieved in graphene-base HETs (GHET). The initial experimental demonstrators of GHETs24-27 showed successful operation in terms of current modulation (on-off ratio >105) but suffered from low output current density (~µA/cm2), low current gain, low injection efficiency, low output impedance and high threshold voltage. These limitations are not intrinsic to the use of graphene as a base material and can be overcome by a careful design and optimization of the device, which are the goals of the present work.
Figure 1. (a) Schematic energy band diagram of a GHET with an insulator-collector barrier along the vertical direction in the on-state for VCB > 0V (solid line) and VCB < 0V (dotted line), showing the carrier flow direction and relevant design parameters. (b) Average base-collector tunneling barrier width for electrons injected in graphene from the emitter as a function of electric field for different base-collector barrier materials. (c) Energy band diagram of the proposed GHET with a graphene/semiconductor Schottky barrier in the on-state for VCB > 0V (dotted line) and VCB < 0V (solid line).
One of the major shortcomings of the GHETs reported so far is the low output current density, which can be increased by improving the i) emitter current (IE) and ii) injection efficiency or base transport factor, defined by:
as shown in the band diagram in Figure 1a, the quantity IE is dominated by the quantum mechanical tunneling of electrons from the emitter to the base. According to the WKB approximation, the tunneling probability (T) through a barrier can be defined as: ∝ , where γ is a function of both the barrier thickness and height. Hence, the emitter current can be significantly increased by scaling the barrier thickness27. However, the initial graphene HETs suffer from a low injection current density from the emitter through the emitter-base barrier due to the thick oxide layers (>5nm SiO2) typically used as the emitter-base barrier24, 25. Narrower tunneling barriers would improve the tunneling probability and also allow a lower turn-on voltage, which would allow the low voltage operation of the device, currently absent in existing HETs (with VBE > 2 V). In the devices reported in this letter (Figure 2a), we use ultrathin AlN on GaN as the emitter stack. The use of all-binary heterostructures eliminates leakage current due to percolation transport arising from random alloy fluctuation28, while the large polarization difference between GaN and AlN enables a very high 2-DEG density in the GaN-side of the heterostructure, which allows for low emitter resistance. Moreover, GaN/AlN heterostructure has
higher tunneling current than Si/SiO2 due to smaller conduction band offset at the junction. The epitaxial nature of the AlN/GaN also provides high quality trap-free interface. To improve the output current density, the common-base injection efficiency, α, should be close to unity. α can be expressed as: = , where αB, αBC and αC represents base efficiency, base-collector barrier filtering efficiency and collector efficiency, respectively. The base efficiency is defined as:
where WB is the physical thickness of the base and λmfp is the carrier mean free path. Monolayer graphene has near unity αB because of its atomically thin nature (t= 3.4 Å) which is superior to any other bulk material. In the case of GaN, the mean free path is around 15 nm29 and αB will be fundamentally limited even in the ultra-scaled base. However, the relatively low values of α in GHETs arise from the poor filtering efficiency (αBC), which will be systematically studied below. The filtering efficiency depends on both the quantum mechanical reflection at the barrier and tunneling conductance of the barrier. To minimize the reflection, base-collector band-offset (ΦBC) should be smaller than the emitter-base band-offset (ΦEB) (Figure 1a), but if ΦBC is too low, then cold electron leakage from the base to the collector will be higher, which will degrade the ballistic injection efficiency. Moreover, to efficiently tune the barrier width with an applied bias and thus modulate the tunneling probability, the barrier shape needs to be triangular rather than trapezoidal27 as for a
trapezoidal barrier, the effective barrier thickness is equal to its physical thickness. Figure 1b shows a comparison of the average tunnel barrier width (computed at the full width at half maximum (FWHM) of the tunnel barrier width) for different conventional dielectrics at the minimum electric field required to change the barrier to a triangular shape from trapezoidal. Owing to the large conduction band offset with graphene (that is 4.5 eV for hBN), the required electric field to achieve a particular tunnel barrier width is relatively large so the device needs to be operated at a relatively large VBC, which makes it prone to breakdown. Therefore, to improve αBC, the base-collector dielectric barrier has to be ultra-thin. Moreover, the base-collector junction in these devices cannot completely screen the emitter electric field which causes severe increase in output conductance. Apart from this fact, forming ultra-thin layers of the dielectrics on a graphene base is very challenging because the chemically inert, hydrophobic surface of graphene does not allow conformal nucleation of atomic layer deposition (ALD) thin film oxides30. Therefore, as a result, relatively thick layers of oxides (~15–55 nm)
24, 25, 27, 31
been used so far to achieve conformal, pin-hole free barriers. Beside their thickness, these dielectrics have relatively large conduction band offsets with graphene (3.3 eV for Al2O3 and 2 eV for HfO2), which cause a dramatic decrease of the current tunneling probability through the barrier and, thus, αBC becomes very poor. Alternatively, one can use a semiconductor instead of an oxide dielectric as the base-collector barrier. Since the semiconductors can typically form a smaller band offset with graphene compared to oxides (for example, ~0.3eV for n-Si15, ~0.5 eV for Ge, ~0.7eV for GaN32), they have a strong band bending effect at the Schottky junction with a metal, which can provide a steep triangular barrier. Therefore, the required field to achieve a given tunnel barrier width is much lower than for insulators (Figure 1b). The doping density and the barrier thickness are additional parameters that can be tuned in semiconductor-based barriers
to further improve αBC. Figure 1c shows the energy band diagram of the proposed HET structure with the graphene/semiconductor heterojunction as the base-collector barrier. The effective tunnel barrier width (WBC) at non-positive VCB (solid line) is large enough to block the tunneling of carriers from the base to collector, similar to a conventional metal/semiconductor heterojunction. In the reverse bias condition (VBC > 0 V), the tunnel barrier width is reduced (dotted lines), therefore the carrier tunneling probability would increase. However, the deposition of conventional semiconductors on graphene encounters the same challenges as the oxides, that is non-uniformity and poor material quality. In this work, we overcame this difficulty by using layered semiconductors from the family of transition metal dichalcogenides (WSe2, MoS2, SnS2 etc.). Thin-films of these materials, as thin as a monolayer, can be easily obtained by mechanical exfoliation owing to weak interlayer van der Waals forces. The atomic layers can then be mechanically transferred on any arbitrary substrate or paired with another atomic layer to form a van der Waals heterojunction with a defect-free, sharp interface. Herein, we propose to use a graphene/WSe2 base-collector junction (Figure 2a), where the graphene-base forms a Schottky barrier to the WSe2 layer. WSe2 is an ambipolar semiconductor with a bulk bandgap of 1.2 eV that increases to 1.6 eV in the monolayer. This configuration would potentially benefit from the small graphene/WSe2 band offset energy (~0.54 eV33), which is in the typical range for a graphene/semiconductor junction. The layered nature of WSe2 enables a thickness control from the monolayer (t ~0.65 nm) to bulk. In this work, we also study the effect of collector layer thickness on the performance metrics of GHET. Figure 2a presents the schematic of the device structure used in this work. We have used a bulk n-GaN (Nd ~ 1019 cm-3) substrate grown by the ammonothermal method to achieve a low threading dislocation defect (TDD) density (<105 cm-2) emitter. A 3 nm AlN tunneling layer was
grown top by plasma-assisted molecular beam epitaxy (details of the growth method are in the Supporting Information). The use of a low TDD density substrate ensures a high film quality and minimal leakage current through the dislocations. A 3 nm GaN layer was used as a capping layer between the AlN and the graphene base..
Figure 2. (a) Schematic cross-section of the fabricated GHET with key terminal voltages. I-V characteristics
(graphene/WSe2/Au) heterojunction diode. Fowler-Nordheim fitting (red dashed line) of the diode I-V characteristics for the B-E diode is shown in the inset. The surface of the as-grown heterostructure was pin-hole free and shows atomic steps with a surface roughness of less than 0.5 nm (the atomic force microscopy image is in the Supporting Information). Electron-beam evaporation was used to deposit an Al film on the back-side to contact the 2-DEG at the AlN/GaN interface through heavily doped n-GaN. To prevent the parasitic conduction between the base and emitter, plasma-enhanced chemical vapor deposition (PECVD) deposited thick SiO2 was used as isolation dielectric (See Figure 2). A monolayer graphene thin film was grown by low-pressure chemical vapour deposition (LPCVD) and then transferred with ethyl-vinyl acetate (EVA) as the supporting polymer [The details of the fabrication method are in the Supporting Information]. The use of EVA ensured the graphene surface had minimal residue from the transfer process34. The transport characteristics of a representative GaN/AlN/graphene diode are shown in Figure 2b. The best performing diode shows a current density of ~ 10 A/cm2 at VBE = 2 V, which is ~150x higher than the highest reported current value for oxide tunnel barriers at the same bias27 (See Supplementary Information for performance comparison of the GaN/AlN B-E barrier with an Al2O3 barrier ). The current density can be further increased by using a thinner barrier with improved film quality. The transport through a tunnel barrier can arise from several potential mechanisms, such as direct tunneling of cold electrons through the barrier, Poole-Frenkel emission through the trap states or Fowler-Nordheim tunneling27. However, both direct tunneling and Poole-Frenkel emission exhibit a very small selectivity for hot electron generation over that for a cold electron,
since carrier transport can occur at any energy in the range from the emitter conduction band to the top of the tunnel barrier. However, the Fowler-Nordheim tunneling mechanism, is highly selective for generating hot electrons at the base27. According to the Fowler-Nordheim model, the current-voltage has the following relationship: − ∝ , where K is a constant dependent on the material parameters, E is the electric field across the barrier and J is the current density. If we plot the diode characteristics as log(I/V2) versus V (Figure 2b(inset)), a good fit is achieved with the Fowler-Nordheim tunneling model at higher VBE, which confirms that the dominant transport mechanism is Fowler-Nordheim tunneling at that bias range and is favorable for hot electron generation. Obviously, the thickness of the B-C barrier is crucial for enhancing the injection ratio of the hot electron carriers from the emitter to the collector and minimizing the background B-C cold current emission.
To evaluate the impact of the WSe2 thickness in our HETs, we fabricated two sets of devices. Device-A: few layer (N=4) WSe2 barrier and device B: 10 nm-thick WSe2 (N~16).
Figure 2c plots the transport characteristics of the B-C diode in device A. The heterojunction was formed by pickup and dry transfer (see the Supporting Information for details) of mechanically exfoliated 4-layer WSe2 flakes on a pre-fabricated B-E stack. The diode characteristics showed a weak rectification with a forward to reverse current ratio of 3 at |VBC|= 1 V. Figure 3a shows the common-base GHET characteristics under different emitter injection currents. The emitter current values were selected considering the current levels obtained in the
B-E diode measurements shown in Figure 2(b). In this configuration, the collector bias was swept while the base was grounded. For negative VCB values in region I (forward bias condition of B-C diode), the injected electrons from the emitter encounter the elevated B-C potential barrier as shown in Figure 3b. As a result, the majority of the electrons contribute to the base current after being reflected by the barrier. Maximum reflection occurs at VCB~ -0.75 V, corresponding to the IC=0 (IB=IE) condition. However, if VCB is gradually increased towards the reverse bias condition of B-C diode (I II), the potential barrier decreases and gradually becomes energetically favorable for the injected electrons to surmount the barrier. This effect is evident in Figure 3a, where the collector current increases from zero to the emitter current level owing to the decreased width of the base collector barrier. Figure 3c plots α at this bias range, which increases from zero to approximately unity. However, if we further increase VCB (region III), the cold electron leakage increases and becomes the dominating component in IC, which explains the upturn in current starting at VBC of approximately 0.3 V.
Figure 3. (a) Common-base characteristics of the device A and (b) corresponding schematic energy band diagrams in different operating regions(c) Injection ratio for device A for different emitter injection currents. Inset shows the Gummel plot for VCB = 0V.
Although this device shows excellent HET characteristics in terms of α, it has a very limited operating VBC window, which suffers from a poor blocking capability of the B-C junction with an ultrathin WSe2 barrier. This limitation arises from the fact that the WSe2 flake used in this device is only 4 atomic layers thick, which allows the hot electron to reach the collector with minimum loss but also, as a blocking barrier, works only for a small bias range (region I and II) with a maximum VCB ~0.3 V. Increasing the number of layers can improve the blocking as the larger interlayer resistance between layers of WSe235 would suppress the cold electron transport between base and collector. Therefore, to achieve a better blocking capability, further optimization of the barrier geometry is required. To understand the effect of the barrier thickness, we increased the WSe2 thickness to 10 nm in device B. The B-C diode characteristics showed that the current through the graphene/WSe2 diode was much smaller (0.5 nA at VCB = 1 V compared with 200 nA in device A) owing to the increased tunneling resistance.
Biasing configuration for electrical characterization of a typical HET. (b) I-V
characteristics of the base-collector diode of device B. Inset shows the same plot on a logarithmic scale (c) IC, IB versus VBE characteristics at different VCB values. (d) Gummel plot in the common-emitter configuration for VCB = 3 V. To characterize the transistor operation, we first biased the device in the common-base mode. Figure 4c plots the base and collector current versus base-emitter voltage at different VCB values. In the absence of an electric field across the B-C junction (VCB = 0 V), the current flow through collector terminal is due to injected carriers from emitter and the current value becomes negligible at VBE =0V. If VCB was increased to higher values, the current magnitude at VBE =2V
shows very small change which indicates that collector current is mainly due to hot electron injection from emitter. However, for lower VBE values we notice a significant increase in the collector current indicating the influence of cold electron leakage (IBC) under these biasing conditions. Next, we biased the device in the common-emitter configuration to study the gain characteristics. Analogous to BJT, the DC current gain (β) in the HET is defined by the following equation in the common-emitter mode:
! = , "
For technological applications, it is important to have the current gain at high current values. Figure 4d plots the simultaneous IC and IB at VCB = 3 V, where the current value is a maximum and we have gain larger than 1. The resultant current gain at VCB = 3 V was found to be ~5.5 at IC = 11 µA (JC
50 A/cm2), which is a record among all graphene-base HETs reported in the
Figure 5. (a) Common-base HET characteristics of the HET at different constant emitter injection currents. The inset compares IBC (the leakage current measured in the two-terminal configuration), IC and IB at IE = 5 µA. (b) Modified injection efficiency in the common-base mode for the characteristics in (a). The inset shows a comparison of the injection efficiencies before and after base-collector cold electron leakage correction as a function of IE.
To understand the origin of the current gain, we characterized the device in the common-base configuration with the emitter terminal used as the constant current source. Since the emitter current value was set to a constant value here, the CB mode measurement could evaluate the hot electron filtering capability of the B-C barrier independent of the B-E heterojunction characteristics. At the low bias regime (VCB < 0.7 V), the collector current was negligible, irrespective of the emitter injection current value. This lower collector current value indicated that all the injected electrons from the emitter get reflected at the B-C interface, and eventually thermalize by scattering at the base where they contribute to the base leakage current. At a higher VCB, the energy barrier of the B-C diode becomes thinner and thus allows the hot electron to pass through the barrier. As a result, the collector current increased monotonically until it reached the emitter current. The inset of Figure 5a compares the base and collector currents at IE = 5 µA and shows a monotonic increase (decrease) of the collector (base) current, which supports the above explanation of the device behavior. Additionally, we should note that using a thicker WSe2 layer in device B allows a larger VCB voltage up to 3 V, compared with 0.3 V in device A. However, increasing the thickness of WSe2 would affect the emission rate of the injected hot electrons as they would have to travel a longer physical path from base to the collector.
The emission rate of the injected hot electrons can be quantitatively evaluated by calculating the common-base injection ratio (α), which represents the ratio of electrons successfully transferred to the collector over the total number of injected electrons from the emitter. Since the emitter current is fixed at a constant value in the CB measurement configuration, the trend of the collector current should represent the value of α which reached to 1 at higher VCB. A unity value of α means all the hot electrons injected from the emitter are being transferred to the collector without being lost in the base owing to scattering or reflection at the C-B barrier (i.e. IC = IEC and IBC= 0). However, at non-zero VCB values, there is a finite current (IBC) flowing between the base and the collector that increases with VCB. The carriers injected from the base to collector are cold electrons, which do not contribute to the amplification. Therefore, calculating α without correcting for B-C leakage overestimates the current gain of the device. Hence, to evaluate the actual amplification potential of the device, we define the ballistic injection efficiency α* to estimate the ratio of electrons quasi-ballistically transferred from the emitter to collector over the total number of injected carriers. To estimate the ballisticity of the device, we subtracted the B-C leakage of the device corresponding to IE = 0 A from the collector current obtained at non-zero emitter current levels and we define the ballistic injection ratio as: α* = (IC−IC(IE = 0 A))/IE 6. Figure 5b shows α* for the same biasing conditions used in Figure 5a. At low VCB, α and α* are essentially the same since the base-collector leakage is negligible. At high VCB biases, the relative increase of α and α* is different owing to the increase of cold electron injection from the base. The ballistic injection efficiency of the present device is a competition between the hot electron transfer and the efficiency from the emitter and the cold electron injection from the base. As a result, α* keeps increasing with VCB until it reaches a peak value where the base collector leakage component starts to dominate the collector current and α* starts to decrease while α
keeps increasing. The maximum value of α* is independent of the injection emitter current level of the emitter, as shown in the inset of Figure 5b. The maximum value of 0.75 indicates that 75% of the injected electrons from the emitter quasi-ballistically travel to the collector terminal, while 25% of the electrons are lost in the base because of reflection. We noted in device A with ultrathin WSe2, α was approximately 100% with the price of a very low operation VCB. We can calculate the current gain (β) in device B using the following formula, similar to the heterojunction bipolar transistor, β = α/(1-α). The maximum β is found to be ~3, which is consistent with the common-emitter mode β obtained in Figure 3. As the comparison of devices A and B shows, the selection of the collector barrier thickness is a trade-off between the tunneling current density and filtering capability of the barrier. Further in-depth studies based of the targeted device application are required to fully optimize the B-C barrier thickness. Additionally, different layered semiconductors can be studied and benchmarked.
Table 1. Benchmarking of different experimental HET performances
We compare the collector current density and DC current gain of different HETs with sub-10 nm base thickness reported in the literature in Table 1. It is evident that the use of a graphene/semiconductor junction improves JC, α and β when compared with the graphene-base oxide collector HETs. (Supplementary Information S5 compares the performance of a graphene/WSe2/Au diode with its counterpart having Al2O3 as the barrier). However, the injection efficiency is still 75% owing to leakage of cold electrons from the base to the collector at the operating condition. A possible solution to enhance the injection efficiency could be the insertion of an ultra-thin insulating hBN tunnel barrier between the graphene and WSe2. The height of the tunnel barrier may prevent the transport of cold electrons near the base conduction band to the collector, while the ultra-thin barrier thickness will add minimal resistance to the energetic hot electrons in the base.
In conclusion, we have demonstrated a graphene-base HET with record performance by using a graphene/WSe2 heterojunction as a base-collector barrier on GaN. This hybrid GaN/vdW HET exhibits JC of 50 A/cm2, β in excess of 3 and α* of 0.75, which can be further improved by a structural and geometric optimization of the device structure. To the best of our knowledge, this work is the first demonstration of the integration of GaN and a van der Waals heterostructure in HETs, and is hoped to lead the way for numerous novel device structures that can be implemented by integrating these two unique material systems. ASSOCIATED CONTENT Supporting Information.
Additional data concerning the AlN growth, device fabrication, graphene growth and transfer, heterostructure fabrication by dry transfer technique and electrical characterization of HET with high-κ dielectric barriers. AUTHOR INFORMATION Corresponding Author *Email: [email protected] ACKNOWLEDGMENT The authors would like to thank Redwan N. Sajjad, Min Sun for helpful discussions on this work and Prof. Pablo-Jarillo Herrero for providing research facilities. This work has been partially supported by the ARO grant No. W911NF-14-2-0071 (monitored by Dr. Joe Qiu), ONR PECASE program, the STC Center for Integrated Quantum Materials, NSF Grant No. DMR1231319, and the AFOSR FATE MURI, Grant No. FA9550-15-1-0514.
REFERENCES 1. Mead, C. A. J Appl Phys 1961, 32, (4), 646-652. 2. Muratake, S.; Watanabe, M.; Suemasu, T.; Asada, M. Electron Lett 1992, 28, (11), 10021004. 3. Heiblum, M.; Thomas, D. C.; Knoedler, C. M.; Nathan, M. I. Applied Physics Letters 1985, 47, (10), 1105. 4. Levi, A. F. J.; Chiu, T. H. Applied Physics Letters 1987, 51, (13), 984-986. 5. Yokoyama, N.; Imamura, K.; Ohnishi, H.; Mori, T.; Muto, S.; Shibatomi, A. Solid State Electron 1988, 31, (3-4), 577-582. 6. Moise, T. S.; Seabaugh, A. C.; Beam, E. A.; Randall, J. N. IEEE Electron Device Letters 1993, 14, (9), 441-443. 7. Yajima, T.; Hikita, Y.; Hwang, H. Y. Nat Mater 2011, 10, (3), 198-201. 8. Tonouchi, M.; Sakai, H.; Kobayashi, T.; Fujisawa, K. Ieee T Magn 1987, 23, (2), 16741677. 9. Dasgupta, S.; Raman, A.; Speck, J. S.; Mishra, U. K. IEEE Electron Device Letters 2011, 32, (9), 1212-1214. 10. Shur, M. S.; Bykhovski, A. D.; Gaska, R.; Khan, M. A.; Yang, J. W. Applied Physics Letters 2000, 76, (22), 3298-3300. 11. Yang, Z. C.; Zhang, Y. W.; Krishnamoorthy, S.; Nath, D. N.; Khurgin, J. B.; Rajan, S. Applied Physics Letters 2016, 108, (19), 192101.
12. Gupta, G.; Ahmadi, E.; Hestroffer, K.; Acuna, E.; Mishra, U. K. IEEE Electron Device Letters 2015, 36, (5), 439-441. 13. Novoselov, K. S.; Mishchenko, A.; Carvalho, A.; Castro Neto, A. H. Science 2016, 353, (6298), aac9439. 14. Britnell, L.; Gorbachev, R. V.; Jalil, R.; Belle, B. D.; Schedin, F.; Mishchenko, A.; Georgiou, T.; Katsnelson, M. I.; Eaves, L.; Morozov, S. V.; Peres, N. M. R.; Leist, J.; Geim, A. K.; Novoselov, K. S.; Ponomarenko, L. A. Science 2012, 335, (6071), 947-950. 15. Yang, H.; Heo, J.; Park, S.; Song, H. J.; Seo, D. H.; Byun, K. E.; Kim, P.; Yoo, I.; Chung, H. J.; Kim, K. Science 2012, 336, (6085), 1140-1143. 16. Mishchenko, A.; Tu, J. S.; Cao, Y.; Gorbachev, R. V.; Wallbank, J. R.; Greenaway, M. T.; Morozov, V. E.; Morozov, S. V.; Zhu, M. J.; Wong, S. L.; Withers, F.; Woods, C. R.; Kim, Y. J.; Watanabe, K.; Taniguchi, T.; Vdovin, E. E.; Makarovsky, O.; Fromhold, T. M.; Fal'ko, V. I.; Geim, A. K.; Eaves, L.; Novoselov, K. S. Nature Nanotechnology 2014, 9, (10), 808-813. 17. Kong, B. D.; Jin, Z.; Kim, K. W. Physical Review Applied 2014, 2, (5), 054006. 18. Di Lecce, V.; Grassi, R.; Gnudi, A.; Gnani, E.; Reggiani, S.; Baccarani, G. Ieee T Electron Dev 2013, 60, (12), 4263-4268. 19. Venica, S.; Driussi, F.; Palestri, P.; Esseni, D.; Vaziri, S.; Selmi, L. Ieee T Electron Dev 2014, 61, (7), 2570-2576. 20. Driussi, F.; Palestri, P.; Selmi, L. Microelectron Eng 2013, 109, 338-341. 21. Mehr, W.; Dabrowski, J.; Scheytt, J. C.; Lippert, G.; Xie, Y. H.; Lemme, M. C.; Ostling, M.; Lupina, G. IEEE Electron Device Letters 2012, 33, (5), 691-693. 22. Di Lecce, V.; Grassi, R.; Gnudi, A.; Gnani, E.; Reggiani, S.; Baccarani, G. Ieee T Electron Dev 2013, 60, (10), 3584-3591. 23. Venica, S.; Driussi, F.; Palestri, P.; Selmi, L. Microelectron Eng 2015, 147, 192-195. 24. Zeng, C.; Song, E. B.; Wang, M.; Lee, S.; Torres, C. M., Jr.; Tang, J.; Weiller, B. H.; Wang, K. L. Nano Lett 2013, 13, (6), 2370-5. 25. Vaziri, S.; Lupina, G.; Henkel, C.; Smith, A. D.; Ostling, M.; Dabrowski, J.; Lippert, G.; Mehr, W.; Lemme, M. C. Nano Lett 2013, 13, (4), 1435-9. 26. Vaziri, S.; Smith, A. D.; Ostling, M.; Lupina, G.; Dabrowski, J.; Lippert, G.; Mehr, W.; Driussi, F.; Venica, S.; Di Lecce, V.; Gnudi, A.; Konig, M.; Ruhl, G.; Belete, M.; Lemme, M. C. Solid State Commun 2015, 224, 64-75. 27. Vaziri, S.; Belete, M.; Dentoni Litta, E.; Smith, A. D.; Lupina, G.; Lemme, M. C.; Ostling, M. Nanoscale 2015, 7, (30), 13096-104. 28. Nath, D. N.; Yang, Z. C.; Lee, C. Y.; Park, P. S.; Wu, Y. R.; Rajan, S. Applied Physics Letters 2013, 103, (2), 022102. 29. Suntrup, D. J.; Gupta, G.; Li, H. R.; Keller, S.; Mishra, U. K. Applied Physics Letters 2014, 105, (26). 30. Nourbakhsh, A.; Adelmann, C.; Song, Y.; Lee, C. S.; Asselberghs, I.; Huyghebaert, C.; Brizzi, S.; Tallarida, M.; Schmeisser, D.; Van Elshocht, S.; Heyns, M.; Kong, J.; Palacios, T.; De Gendt, S. Nanoscale 2015, 7, (24), 10781-10789. 31. Lan, Y. W.; Torres, C. M., Jr.; Zhu, X.; Qasem, H.; Adleman, J. R.; Lerner, M. B.; Tsai, S. H.; Shi, Y.; Li, L. J.; Yeh, W. K.; Wang, K. L. Sci Rep 2016, 6, 32503. 32. Tongay, S.; Lemaitre, M.; Schumann, T.; Berke, K.; Appleton, B. R.; Gila, B.; Hebard, A. F. Applied Physics Letters 2011, 99, (10), 102102. 33. Kim, K.; Larentis, S.; Fallahazad, B.; Lee, K.; Xue, J. M.; Dillen, D. C.; Corbet, C. M.; Tutuc, E. Acs Nano 2015, 9, (4), 4527-4532.
34. Hong, J. Y.; Shin, Y. C.; Zubair, A.; Mao, Y.; Palacios, T.; Dresselhaus, M. S.; Kim, S. H.; Kong, J. Adv Mater 2016, 28, (12), 2382-92. 35. Das, S.; Appenzeller, J. Phys Status Solidi-R 2013, 7, (4), 268-273. 36. Torres, C. M., Jr.; Lan, Y. W.; Zeng, C.; Chen, J. H.; Kou, X.; Navabi, A.; Tang, J.; Montazeri, M.; Adleman, J. R.; Lerner, M. B.; Zhong, Y. L.; Li, L. J.; Chen, C. D.; Wang, K. L. Nano Lett 2015, 15, (12), 7905-12.